Table 82. Continued. 











Corrosion 





Alloy 



Environment' 7 



Exposure 



(day) 



Depth 

 (ft) 





Source 6 



Rate 



(mpy) 



Type 6 



75A 



W 



588 



5 



0.0 



NC 



CEL (4) 



75A' V 



W 



588 



5 



0.0 



NC 



CEL (4) 



75A l? 



W 



588 



5 



0.0 



NC 



CEL (4) 



0.15 Pd J 



w 



189 



5,900 



0.0 



NC 



CEL (4) 



0.15 Pd* 



w 



189 



5,900 



0.0 



NC 



CEL (4) 



0.15 Pd rf 



s 



189 



5,900 



0.0 



NC; BD 



CEL (4) 



0.15 Pd e 



s 



189 



5,900 



0.0 



NC; BD 



CEL (4) 



0.15 Pd'^ 



w 



181 



5 



0.0 



NC; FS 



CEL (4) 



0.15 Pd ? 



w 



181 



5 



0.0 



NC;FS 



CEL (4) 



0.15 ?d d 



w 



398 



5 



0.0 



NC 



CEL (4) 



0.15 Pd'' 



w 



398 



5 



0.0 



NC 



CEL (4) 



0.15 Pd rf 



w 



540 



5 



0.0 



NC 



CEL (4) 



0.15 Pd* 



w 



540 



5 



0.0 



NC 



CEL (4) 



0.15 Pd' f 



w 



588 



5 



0.0 



NC 



CEL (4) 



0.15 Pd* 



w 



588 



5 



0.0 



NC 



CEL (4) 



5Al-2.5Sn rf 



w 



123 



5,640 



<0.1 



NC 



CEL (4) 



5AI-2.5Sn e 



w 



123 



5,640 



0.0 



NC 



CEL (4) 



5Al-2.5Sn d 



s 



123 



5,640 



<0.1 



NC 



CEL (4) 



5Al-2.5Sn e 



s 



123 



5,640 



0.0 



NC 



CEL (4) 



5Al-2.5Sn J 



w 



189 



5,900 



0.0 



NC 



CEL (4) 



5Al-2.5Sn* 



w 



189 



5,900 



0.0 



NC 



CEL (4) 



5Al-2.5Sn'' 



s 



189 



5,900 



0.0 



NC; BD 



CEL (4) 



5Al-2.5Sn e 



s 



189 



5,900 



0.0 



NC; BD 



CEL (4) 



5Al-2.5Sn d 



w 



403 



6,780 



0.0 



NC 



CEL (4) 



5Al-2.5Sn e 



w 



403 



6,780 



0.0 



NC 



CEL (4) 



5Al-2.5Sn rf 



s 



403 



6,780 



0.0 



NC 



CEL (4) 



5Al-2.5Sn e 



s 



403 



6,780 



0.0 



NC 



CEL (4) 



5AI-2.5Sn d 



w 



751 



5,640 



0.0 



NC 



CEL (4) 



5Al-2.5Sn e 



w 



751 



5,640 



0.0 



NC 



CEL (4) 



5Al-2.5Sn d 



w 



197 



2,340 



0.0 



NC 



CEL (4) 



5Al-2.5Sn ? 



w 



197 



2,340 



0.0 



NC 



CEL (4) 



5Al-2.5Sn rf 



s 



197 



2.340 



0.0 



NC 



CEL (4) 



5Al-2.5Sn f 



s 



197 



2,340 



0.0 



NC 



CEL (4) 



5Al-2.5Sn d 



w 



402 



2,370 



0.0 



NC 



CEL (4) 



5Al-2.5Sn* 



w 



402 



2,370 



0.0 



NC 



CEL (4) 



5Al-2.5Sn J 



s 



402 



2,370 



0.0 



NC 



CEL (4) 



5Al-2.5Sn e 



s 



402 



2,370 



0.0 



NC 



CEL (4) 



5Al-2.5Sn rf 



w 



181 



5 



0.0 



NC; FS 



CEL (4) 



5Al-2.5Sn e 



w 



181 



5 



0.0 



NC; FS 



CEL (4) 



Continued 



229 



